Download presentation

1
CHAPTER 2: PLASTICITY

2
**CHAPTER 2: PLASTICITY AISI 1040 Steel Yield stress varies 250-1100MPa**

Total Strain varies between Properties of steel depend on heat treatment and quenching produces a hard martensitic structure which is gradually softened by tempering at higher temperatures. The annealed structure is ductile but has low yield stress. The ultimate tensile stresses are marked by arrows. After these points plastic deformation becomes localized (called necking) and the engineering stresses drop because of the localized reduction in the cross sectional area. However true stress continues to rise because the cross sectional area decreases and material work hardens in the neck region. True stress-true strain curves are obtained by converting the tensile stress and its corresponding strain values into true stress and extending the curve.

3
**CHAPTER 2: PLASTICITY Volume stays constant**

The incremental longitudinal strain:

4
CHAPTER 2: PLASTICITY

5
**CHAPTER 2: PLASTICITY n<1 Parabolic hardening**

Translate it upward by assuming yield stress is equal to σ0 then equation becomes: n is called strain hardening exponent and depends on the nature of the material, the temperature at which it is work hardened and strain. n varies between 0.2 and 0.5 and K is in between G/100 and G/1000. The equations predict a slope of infinity for ε=0 which does not conform experimental results. The equations imply that σ→∞ when ε→∞ ( We know this is not correct and that experimentally a saturation of stress occurs at higher strains.

6
CHAPTER 2: PLASTICITY The fact that some equations reasonably approximate the stress-strain curves does not imply that they are capable of describing the curves in a physically satisfactory way. There are two reasons for this: (1) In the different position of stress-strain curves, different microscopic processes predominate. (2) Plastic deformation is a complex physical process that depends on the path taken; it is a thermodynamic state function. The accumulated is not uniquely related to the dislocation structure of the material. Ludwik-Hollomon is the most common representation of plastic response. When n=0, it represents ideal plastic behavior (no work-hardening). More general forms of this equation, incorporating both strain rate and thermal effects, are often used to represent the response of metals; in that case they are called constitutive equations. The flow stress of metals increases with increasing strain rate and decreasing temperature because thermally activated dislocation motion is inhibited.

7
CHAPTER 2: PLASTICITY

8
**CHAPTER 2: PLASTICITY A=0.2% offset yield stress**

B and C= upper and lower yield point D=proportional limit (stress at which the curve deviates from linearity) D’=UTS E=rupture stress F=Uniform Strain Beyond F necking starts G is strain to failure. Elastic energy absorbed=Resilience=area under elastic portion of the curve Work of fracture= Total area under the curve

9
CHAPTER 2: PLASTICITY

10
CHAPTER 2: PLASTICITY

11
CHAPTER 2: PLASTICITY

12
CHAPTER 2: PLASTICITY

13
CHAPTER 2: PLASTICITY

14
CHAPTER 2: PLASTICITY

15
CHAPTER 2: PLASTICITY

16
CHAPTER 2: PLASTICITY

17
CHAPTER 2: PLASTICITY

18
CHAPTER 2: PLASTICITY

19
CHAPTER 2: PLASTICITY

20
CHAPTER 2: PLASTICITY

21
CHAPTER 2: PLASTICITY

22
CHAPTER 2: PLASTICITY

23
CHAPTER 2: PLASTICITY

24
CHAPTER 2: PLASTICITY

25
CHAPTER 2: PLASTICITY

26
CHAPTER 2: PLASTICITY

27
CHAPTER 2: PLASTICITY

28
CHAPTER 2: PLASTICITY BAUSCHINGER EFFECT

29
CHAPTER 2: PLASTICITY

30
CHAPTER 2: PLASTICITY

31
CHAPTER 2: PLASTICITY

32
CHAPTER 2: PLASTICITY

33
CHAPTER 2: PLASTICITY

34
CHAPTER 2: PLASTICITY

Similar presentations

Presentation is loading. Please wait....

OK

NEEP 541 – Creep Fall 2002 Jake Blanchard.

NEEP 541 – Creep Fall 2002 Jake Blanchard.

© 2019 SlidePlayer.com Inc.

All rights reserved.

To make this website work, we log user data and share it with processors. To use this website, you must agree to our Privacy Policy, including cookie policy.

Ads by Google